Manufacturable AlSb/InAs HEMT Technology for Ultra-Low Power Millimeter- Wave Integrated Circuits R. Tsai1, R. Grundbacher1, M. Lange1, J. B. Boos2, B. R. Bennett2, P. Nam1, L. J. Lee1, M. Barsky1, C. Namba1, K. Padmanabhan1, S. Sarkozy1, P. H. Liu1, and A. Gutierrez1 1 Northrop Grumman Space Technology, Inc., Redondo Beach, CA 90278 Tel: (310) 812-8254, Fax: (310) 813-0418, Email: firstname.lastname@example.org 2 Naval Research Laboratory, Washington, DC 20375-5320, USA Abstract Northrop Grumman Space Technology (NGST) and Naval High electron mobility transistors with InAs channels and Research Laboratory (NRL) for ultra low-power, high sub 0.1-Pm metal gates, have demonstrated a 100% frequency MMIC products. improvement in low-power, high-speed figure of merits over conventional InAlAs/InGaAs lattice-matched HEMTs and MHEMTs. AlSb/InAs MHEMTs exhibit transconductances as high as 1.3 S/mm at drain biases as low as 0.3 V, while InAlAs/InGaAs HEMT & MHEMT: 75 mW/mm maintaining fT and fmax results greater than 220 GHz and 270 GHz, respectively. In this paper, we will discuss our efforts to AlSb/InAs HEMT: 6 mW/mm develop this technology for revolutionary low-power, high 600 Gate Voltage frequency MMIC applications. Steps of 0.1 V Drain Current (mA/mm) 500 INTRODUCTION 400 Monolithic Millimeter-wave Integrated Circuits (MMIC) based upon InAs-channel HEMT’s have the potential to enable revolutionary low-noise, low-power, and high-speed 300 applications. As shown in Table 1, InAs electronic properties, such as electron mobility and peak velocity, are 200 nearly two times larger as compared to state-of-the-art InXGa1-XAs-channels. 100 InAlAs/InGaAs HEMT’s grown on lattice-matched InP substrate offer the best combination of low-power and low- 0 noise MMIC’s to date [1-2]. Based on our device data, as 0 0.25 0.5 0.75 1 shown in Figure 1, we estimate InAs-based HEMT performance meets or exceeds InAlAs/InGaAs HEMT but Drain-Source Voltage (V) with only one-tenth the power dissipation. Fig. 1 AlSb/InAs HEMT (solid) bias points for minimum noise figure and However, development of InAs channel devices is lowest DC power dissipation, compared to InAlAs/InGaAs HEMT challenging because of the lack of viable semi-insulating (dashed). Curves displayed for gate voltage step of 0.1 V. substrates for lattice-matched growth. Metamorphic growth using the AlXGa1-XSbYAs1-Y/InAs material system, which has a lattice constant near 6.1 Å, as shown in Figure 2, has Table 1. HEMT Channel Electron Transport Properties proven to be a viable alternative for state-of-the-art InAs- channel HEMTs [3-5] and researchers in this field now Property InAs In0.53Ga0.47As GaAs m e* 0.023 0.041 0.067 routinely achieve electron mobility > 15,000 cm2/V-s with µ (cm /V-sec) 2 20000 8000 4500 tensile strained InAs channels. However, the approach does Peak velocity 4.0 2.7 2.2 hold several unique challenges such as intrinsic material 7 (10 cm/sec) stability, gate leakage, and yield limiting defect densities, Γ-L valley 0.9 0.55 0.31 which have been incrementally addressed over the years . seperation (eV) Only recently have the first AlSb/InAs MHEMT based Band Gap (eV) 0.36 0.72 1.42 MMIC’s been demonstrated [7,8]. In this paper, we will discuss the successful development of a manufacturable AlSb/InAs MHEMT technology at 2.8 0.45 production MBE reactors is a testament to its AlP ZnSe reproducibility. Detailed technical rationale regarding the 0.50 2.4 AlAs ZnTe implementation of the hole barrier, doping plane, and buffer Energy Gap (eV) Wavelength (µm) 2.0 GaP 0.60 cap in our standard profile can be found in previous publications [3,4,9]. AlSb 1.6 0.80 Furthermore, by optimizing MBE flux conditions and InP modulation doped methodology, the same profile obtains an GaAs 1.00 1.2 Si average sheet resistance of 200.9 Ω/sq with less than 2.6% 1.30 0.8 In G GaSb non-uniformity and 300K mobility of 26,300 cm2/V*s with aA s 2.00 electron sheet density of 1.28x1012 cm-2, as shown in the Ge InAs 0.4 trend chart of Figure 4. This combination of over 30% 5.00 higher mobility and lower sheet charge provides better 0 InSb 5.4 5.6 5.8 6.0 6.2 6.4 characteristics for ultra-low power circuit applications. The Lattice Constant (Å) device pinch off voltage becomes more positive, while access resistance increases only marginally. Fig. 2 The AlXGa1-XSbYAs1-Y/InAs material system and approximate 6.1 Å lattice constant 35000 800 30000 700 Hall Mobility (cm/V*s) DEVICE GROWTH & FABRICATION Sheet Resistance 25000 600 2 (Ohms/sq) The AlSb/InAs structures were grown by molecular beam epitaxy (MBE) on semi-insulating 3” GaAs substrates, 20000 500 and both NGST and NRL labs have grown several wafers of 15000 400 a standard structure, as shown in Figure 3, to qualify the transference of growth and frontside process methodology, 10000 300 as well as comparative analysis. 5000 200 0 100 0 10 20 30 40 50 Growth Run Fig. 4 Statistcal process control data for 50 epitaxially grown 3” wafers (Triangles) 300 K electron hall mobility (Squares) sheet resistance. NGST’s fabrication process uses qualified InP-HEMT production optical-stepper lithography, cleaning procedures, SPCM testing, and database tracking. Active device mesas were formed by using a BCl3/Ar-based Inductively-coupled Plasma (ICP) etch to remove 1250 Å of the structure. The mesa isolation process was designed to end in the Al0.7Ga0.3Sb layer, and achieves an average of 100 MΩ/sq of Fig. 3 Layer structure of one standard profile grown at NGST and NRL electrical isolation resistance without the need for implant isolation. This level of isolation is comparable to NGST’s space-qualified, production InAlAs/InGaAs/InP HEMT’s Both labs schedule destructive Hall measurements of as- that employs both mesa isolation and implant isolation. grown standard profile wafers and perform non-destructive Pd/Pt/Au ohmics alloyed at 175°C in a nitrogen atmosphere sheet resistance mapping on every grown wafer for formed contacts with a resistance of 0.06 Ω-mm. Electron statistical process control monitoring (SPCM). According to beam lithography was utilized to fabricate 0.1 µm Mo/Au T- SPCM statistics, our standard profile grown obtains an gates in a 2 µm source-drain region. The source to gate average sheet resistance of 180.5 Ω/sq with less than 2.6% distance was 0.8 µm. non-uniformity and 300K mobility of 19,100 cm2/V*s with Our MMIC integration process is identical to our flight- electron sheet density of 1.77x1012 cm-2. The fact that state- qualified InAlAs/InGaAs/InP HEMT process . This of-the-art growth of AlXGa1-XSbYAs1-Y/InAs HEMT profiles process features devices and passive circuit components can be successfully controlled in both research and pre- which are fully passivated with a total of 750 Å PECVD SiN, two levels of interconnect metal including airbridges, 1000 Top Curve: Gate Voltage of 0 V 300 pF/mm2 double-layer MIM capacitors with breakdown Steps of -0.05 V voltages over 100 volts, and 100-Ω/sq precision NiCr Drain Current (mA/mm) 800 resistors with 0.6 mA/µm reliable operation. Upon completion of frontside processing, wafers were 600 thinned to a thickness of 100 µm. Round 40 µm diameter vias were etched through the substrate to allow contact from the HEMT source pads to the backside wafer ground plane. 400 200 RESULTS & DISCUSSION 0 Devices were DC tested on-wafer at the completion of 0 0.1 0.2 0.3 0.4 0.5 processing. The devices displayed high transconductance (GM) at low drain-source voltage (VDS), and low on-state Drain-Source Voltage (V) resistance (RON). The average GM peak was 1.05 S/mm and 2.56 S/mm measured at a VDS of 0.2 V and 0.4 V 400 2500 TOP CURVE: Vds = 0.4 V DC Transconductance (mS/mm) respectively. The average off-state reverse gate-drain 350 breakdown (BVGDR) was –1.42 V (measured at a gate current STEPS OF -0.1 V 2000 300 of -1 mA/mm). An example of the DC drain current (ID) versus drain voltage (VD) is shown in the top of Figure 5, 250 1500 while GM vs. gate voltage (VG) is shown in the bottom. DC fT (GHz) 200 characteristics in Figure 5 were measured from a 2-fingered 1000 80-µm total gate periphery device, and illustrate the 150 combined characteristics of low drain voltage operation, low 100 500 knee voltage, and high transconductance, which are critical 50 parameters for ultra-low power, high frequency operation. Device functional yields as high as 97% have been achieved 0 0 -0.8 -0.7 -0.6 -0.5 -0.4 -0.3 -0.2 -0.1 0 for 3” wafers with excellent uniformity of DC characteristics, as depicted in Figure 6. Gate Voltge (V) Small signal RF tests were also performed on-wafer, and maximum available gains greater than 10 dB at 100 Fig. 5 Top: Measured drain current vs. drain voltage and Bottom: Extrapolated unity current gain frequency (dashed) and measured DC GHz and fmax higher than 270 GHz were measured starting at transconductance (solid) vs. gate voltage. VDS of 0.4 volts and 112 mA/mm, as shown in Figure 7. 30 MAG Maximum Gain (dB) 25 20 15 10 5 0 1 10 100 Frequency (GHz) Fig. 6 Device yield of forty 4 x 75-µ m devices across a 3” wafer depicted Fig. 7 Measured maximum available gain greater than 10 dB at 100 GHz as location dependent DC-IV plots. Also drawn are four large-area hall bar, for 2 x 40-µ m devices. and four plating clip dropouts, and non-functional devices as “X”. The average peak fT, was 153 GHz and 212 GHz at VDS 20 4 of 0.2 and 0.4 volts and drain current densities of 115 and 17.5 3.5 Assosciated Gain (dB) 340 mA/mm, respectively. These correspond to DC power dissipations of 22 and 180 mW/mm. Compared to fT-DC power performance of state-of-the art 0.1-µm gate length 15 3 InAlAs/InGaAs/InP HEMT’s, our AlSb/InAs HEMT’s 12.5 2.5 FMIN (dB) provide equivalent high-speed figure of merit performance at 5 to 10 times lower power dissipation, as shown in Figure 8. 10 2 7.5 1.5 250 5 1 200 Increasing Vds 2.5 0.5 0 0 150 0 5 10 15 20 25 30 fT (GHz) 100 Frequency (GHz) Fig. 9 Measured 2 to 26 GHz associated gain (G A) and minimum noise 50 figure (FMIN) at VDS = 0.2 volts and 6 mW/mm DC power dissipation. 0 1 10 100 1000 REFERENCES DC Power Dissipation (mW/mm)  R. Raja, et al., 2001 IEEE MTT-S Technical Digest, pp. 1955-1958, 2001. Fig. 8 Extrapolated unity current gain frequency vs. DC power dissipation  R. Lai, et al., Proceedings of 2000 International Electron Devices for AlSb/InAs HEMT (solid) at VDS = 0.1, 0.2, and 0.5 volts and Meeting, pp. 175-177, 2000. InAlAs/InGaAs HEMT (dashed) at VDS = 0.2, 0.5, and 1.0 volts.  J. B. Boos, et al., IEEE Trans. Electron Device, vol. 45, no. 9, pp. 1869- 1875, 1998. Noise-pull tests were also performed on-wafer. As shown in Figure 9, at an ultra-low power dissipation bias of  J. B. Boos, et al., Electronics Letters, vol. 34, no. 4, pp. 403-404, 1998. 6 mW/mm a minimum noise figure of 0.85 dB and  K. Yoh, et al., IEEE Electron Device Letters, vol. 11, no. 11, pp. 526- associated gain of 11.5 dB was measured at VDS of 0.2 volts. 528, 1990. These minimum noise figures are comparable to state-of-art GaAs and InAlAs/InGaAs/InP HEMT’s up to 26 GHz, but at  C. R. Bolognesi, Proceedings of 14th Indium Phosphide and Related Materials Conf., pp. 55-58, 2002. 10 times lower power dissipation.  J. Bergman, et al., 53rd Device Research Conference, presentation, 2003. CONCLUSIONS  R. Tsai, et al., Technical Digest of 2003 IEEE GaAs IC Symposium, pp. 294-297, 2003. NGST and NRL have demonstrated a high performance and highly reproducible AlSb/InAs HEMT technology with  R. Tsai, et al., Proceedings of IEEE Lester Eastman Conf. on High revolutionary combined ultra-low power dissipation and Performance Devices, pp. 276-280, 2002. excellent high-frequency performance.  Y. C. Chou, et al., Technical Digest of 2002 IEEE GaAs IC Symposium, pp. 77-80, 2002. ACKNOWLEDGEMENTS This work was supported by ONR Cooperative Agreement No.: N00014-01-2-0014, DARPA ABCS Program. The authors would like to thank Colin Wood (ONR), Don Mullin and Cynthia Hanson (SPAWAR), and Mark Rosker (DARPA).